intro composite applns. properties voigt, reuss, hill anistrpy. cte cellular matls. wood 1...
Post on 29-Dec-2015
Embed Size (px)
Microstructure-Properties Lecture 1: What is Microstructure?
1Microstructure-Properties: CompositesMicrostructurePropertiesProcessingPerformance27-301A. D. Rollett, M. De GraefLast modified: 27th Sept. 15
2Lecture Objectives: CompositesThe main objective of this lecture is to introduce you to microstructure-property relationships in composite materials.Composite materials constitute a huge class of materials. The objective of this lecture will therefore be to provide some definitions and describe some of the basic relationships.Cellular materials will be emphasized because of their connection to natural materials (biomaterials) and especially wood, which some of you will study in the second Lab.
12 Questions for Part 1What are the general advantages of composite materials over monolithic materials? Give both biomaterial and man-made examples. Composites generally have higher specific properties. Wood and carbon-fiber reinforced plastics are examples.What is the rule of mixtures as applied to composites? Integrate the property of interest over the volume of the composite.What do the terms isostress and isostrain mean? As implied, iso-stress means same stress in all materials; iso-strain means same strain in all materials. For iso-stress you can think of the phases as being connected in series between the planes across which the load is transmitted (and vice versa for iso-strain).Derive the isostrain model. See the notes; derivation relies on averaging the stresses in the different phases. Derive the isostress model. See the notes; derivation relies on averaging the strains in the different phases.Sketch the variations in modulus expected for composites in which the components have strongly different moduli. See the notes; iso-strain model gives linear variation (same as Rule of Mixtures in this case) whereas iso-stress model gives non-linear variation.Explain what is meant by the Voigt, Reuss and Hill average moduli. Voigt=iso-strain, Reuss=iso-stress, Hill averages these two.Describe the multiscale microstructure of wood. See the notes; one can start at the level of the cellulose bundles and work up through cells to the structure of the trunk.Explain the structure and components of micro-fibrils. Each microfibril is a bundle of cellulose fibers in a matrix of hemicellulose and lignin. Explain the structure of cell walls in wood. See the notes; Several layers present in the cell wall, each with its own characteristic lay-up angle of the micro-fibrils.Describe the anisotropy of the elastic stiffness of wood. Wood is much stiffer parallel to the grain.Based on the chemistry of wood, comment on its sensitivity to moisture. Certain components of the wood (esp. cellulose) are hydrophilic and absorb water. Increased moisture content increases stiffness and strength.3IntroCompositeApplns.PropertiesVoigt, Reuss,HillAnistrpy.CTECellularMatls.Wood
4Key pointsComposites are regarded as artificial (man-made) mixtures of phases.Classification of composites by reinforcement type (dimensionality) - particles, fibers and laminated.Application of the Rule of Mixtures.Dependence of composite properties on the spatial arrangement of the phases.Upper and lower bounds on properties - example of elastic modulus, Voigt and Reuss approximations.High property:density ratios achievable with composites.Engineering with residual stress in composites.Anisotropy of composite properties, e.g. elastic modulus.Properties of wood as a cellular material.Cellular/foam materials as shock absorbers.ExaminableIntroCompositeApplns.PropertiesVoigt, Reuss,HillAnistrpy.CTECellularMatls.Wood
6What are Composites?Composite materials contain more than one phase.Almost all materials contain more than one phase, so whats the difference?The term composite is typically applied to a material when the multi-phase structure is constructed by direct intervention (external to the material). Composite Material Examples: glass fiber reinforced plastic (GRP), wood, clam shell, Mars bar.Multi-phase Material Examples: precipitation strengthened aluminum alloys, Ti-6Al-4V, dual-phase steel, transformation toughened alumina (Al2O3-CeO2).Caution! There is some overlap between the categories!ExaminableIntroCompositeApplns.PropertiesVoigt, Reuss,HillAnistrpy.CTECellularMatls.Wood
7PropertiesIt is useful to review the basic properties of the different types of materials that are used in composites.Polymers - long [carbon] chain molecules with anything from van der Waals bonding between the chains (thermoplastics) to covalent links (thermosets). Low density, low modulus compared to other materials. Often highly formable (ductile).Ceramics - ionic or covalent bonding, lower symmetry crystal structures, high melting point and modulus, resistant to degradation, brittle, high modulus.Metals - metallic bonding, symmetric crystal structures, medium melting point, medium modulus, ductile, formable, variable resistance to degradation.ExaminableIntroCompositeApplns.PropertiesVoigt, Reuss,HillAnistrpy.CTECellularMatls.Wood
8Why Use Composites? [Biomaterials]In nature, the basic materials tend to be weak and/or brittle. Evolution has resulted in structures that combine materials together for properties that far exceed those that could be obtained in the basic materials. The basic inorganic constituent of bone, for example, is calcium phosphate in the form of crystalline Ca10(PO4)6(OH) and amorphous CaPO3. This ceramic is brittle and not particularly stiff. The matrix of fibrous collagen is tough but even less stiff. When embedded arranged in the form of a cellular material, however, remarkable values of stiffness:density and toughness:density are achieved (and land-based multi-tonne creatures are possible such as elephants).A similar situation exists in wood where the basic materials are quite compliant but arranged in the multi-level composite forms that we know, high values of strength:density and toughness:density result.IntroCompositeApplns.PropertiesVoigt, Reuss,HillAnistrpy.CTECellularMatls.Wood
9Why Use Composites? [Man-made]The basic reason for the use of composites is always the same: some combination of properties can be achieved that is impossible in a monolithic material [for a given cost].In SiC-reinforced aluminum for brake rotors, for example, the combination of light weight, toughness (from the Al matrix at ~ 2.7 Mgm/m3), and stiffness (from the SiC additions) is not possible in either constituent by itself.In Cu-Nb for high strength electrical conductors, the combination of >1GPa yield strength and high electrical conductivity (in the Cu) could never be achieved in either constituent by itself. In this case the high strength is a synergistic property of the composite.IntroCompositeApplns.PropertiesVoigt, Reuss,HillAnistrpy.CTECellularMatls.Wood
10Key aspects of compositesComposites are expensive to make, as compared to monolithic materials, especially if the shape and arrangement of the phases must be controlled.Therefore there must be a strong motivation for making a composite structure to offset the cost.The simplest composites are particulate composites. Laminates are next, followed by fiber composites. Woven structures are the most complex.ExaminableIntroCompositeApplns.PropertiesVoigt, Reuss,HillAnistrpy.CTECellularMatls.Wood
11Typical MicrostructuresWe show next some typical microstructures.In biomaterials, many are cellular composites at some length scale (typically around 1 m).Man-made composites are more often fully dense. The three major [structural] material types are all used so the abbreviations MMC [metal matrix composite], CMC [ceramic matrix composite], and PMC [polymer matrix composite] are commonly used.ExaminableIntroCompositeApplns.PropertiesVoigt, Reuss,HillAnistrpy.CTECellularMatls.Wood
Gibson & Ashby: Cellular SolidsNote the variation in density; also the presence of distinct layers of cells in some woods, and in bone.
Note also that the shape of the cells and their walls makes a difference to their properties.IntroCompositeApplns.PropertiesVoigt, Reuss,HillAnistrpy.CTECellularMatls.Wood
SiC fibers in Ti3Al matrixSiC fibers in a CAS ceramic matrixDowling: Mech. Beh. Matls.Note the typical length scale of ~100m, and the use of fibers for reinforcement. This basic type of fiber-reinforced composite is strongly anisotropic. The toughness of such composites and the need for limited adhesion between fiber and matrix was discussed in the lecture on Fracture.IntroCompositeApplns.PropertiesVoigt, Reuss,HillAnistrpy.CTECellularMatls.Wood
From left to right, top to bottom:a) Breadb) Meringuec) Chocolate bard) Chipe) Malteser (Candy)f) Jaffa cake (cookie, see below)Gibson & Ashby: Cellular Solids
Maltesers image: commons.wikimedia.org/MaltesersOpen.jpgJaffa: thetastingbuds.comIntroCompositeApplns.PropertiesVoigt, Reuss,HillAnistrpy.CTECellularMatls.Wood
15Food for Thought!How does ice cream represent a material in which the thermal-mechanical history is critical to its microstructure which, in turn, controls its properties?IntroCompositeApplns.PropertiesVoigt, Reuss,HillAnistrpy.CTECellularMatls.Wood
16Examples of compositesThe classical example of a composite is concrete.It is more complex than it appears. There are typically coarse and fine particles (rocks!) embedded in a matrix of silicates and sulfates. There is a high fraction of pores of all sizes. This is an example of a particulate composite.Ordinary concrete (properly made) has e